Surface and Sliding Wear Behaviour of Different Coatings and Steels
Resistencia al desgaste por deslizamiento de diferentes recubrimientos y aceros
Información del artículo: recibido: julio de 2010, reevaluado: octubre de 2010, aceptado: febrero de 2011
Universidad Politécnica de Pachuca, Zempoala Hgo., México Correo: email@example.com
Instituto Politécnico Nacional, México DF Correo: firstname.lastname@example.org
University of Sheffield, Department of Mechanical Engineering, United Kingdom
In this work, the sliding wear behaviour of the coatings TiN, CrN and WC/C applied on steel substrates was studied using a reciprocating wear test ma-chine. All tests were carried out in dry conditions, at room temperature (20-23°C and 45%−50% relative humidity). The average sliding velocity was 0.08 m/s and an amplitude of 2 mm was used. The applied loads were 11.76 N (Po = 1.74 GPa) and 7.84 N (Po = 1.52 GPa). Optical microscopy was used to ob-serve the characteristics of wear scars and spalls and possible causes of their formation. The variation of the friction coeﬃ cient against the number of cy-cles was obtained. This was used to determine more precisely the time (num-ber of cycles) where the coating presented the fi rst signs of wear, in addition Energy Dispersive X-ray analysis (EDS) was performed, as well as Scanning Electron Microscopy (SEM) and hardness tests on the wear traces, which reinforced the previous observations. Thus it was possible to know the wear life of diﬀ erent coatings and possible causes of variation. Increasing the load was an important factor in the variation of wear life results. But it is also important to consider other factors such as surface roughness and thickness of coatings.
• wear • substrate
Hard surface coatings have shown good performance in applications such as coating of cutt ing tools, stam-ping processes and forming and plastic injection tooling, amongst others (Vera et al., 2008). The aim of the present work was to study the wear and friction behaviour of coatings TiN, CrN and WC/C, when ex-posed to dry sliding conditions.
Diﬀ erent standard substrate materials for applica-tions in bearings and gears were studied. It was of in-terest to know the wear performance of these coatings when sliding in dry conditions and with substrate ma-terials not common in the literature (4320 steel, 8620 steel and 4140 steel).
One of the steels currently most commonly used in alloys for cutt ing tools and bearings is 100Cr6 steel. It is intended to fi nd other alternatives in the types of steel that can be used for the applications mentioned when a thin fi lm hard coating is applied to improve its wear resistance.
A great deal of research work about sliding wear and friction with coatings involves 100Cr6 (AISI 52100) steel as a substrate material (Srikant et al., 2004). Tungsten car-bide coatings have been applied to improve the life of extrusion dies, metrology parts and bearings. The micro-hardness ranges from 800 to 2100 HV. The properties such as microhardness and stoichiometry are strongly
infl uenced by the deposition parameters (Bhusham et al., 1991). For soft fi lms on hard substrates the load capacity decreases as fi lm thickness increases, while for hard
fi lms on soft substrates the converse is true (Arnell et al., 1991). Some of the work carried out associated with the use of hard coatings is shown in table 1.
A reciprocating wear tester was used to carry out ball-on-fl at wear tests. The tester holds the ball specimens in a clamp on the reciprocating arm and fl at disc speci-mens in a base unit via another clamp. The reciprocator (LDS V201 vibrator) is controlled by a function genera-tor. Friction measurements were taken via a load cell SM-50N model, with a capacity of 50 N and a nominal rated output of 3mV/V. Figure 1 shows a photograph of the wear tester (Green et al., 2005).
The disc specimens have a diameter of 19 mm and a thickness of 3.5 mm. The characteristics of the steel substrates and coatings used are shown in the table 2. A 100Cr6 steelball (diameter 4.75 mm) was used. The coa-tings were applied by Oerlikon Balzers in Mexico. They were deposited with the PVD technique in a BAI 1200 machine with a high vacuum and at a temperature about 450°C.
En este trabajo se estudió el comportamiento en desgaste por deslizamiento de los recubrimientos de TiN, CrN y WC/C aplicados sobre sustratos de acero. Las prue-bas se realizaron con una máquina reciprocante en condiciones secas a tempera-tura ambiente (20-23°C y 45%−50% de humedad relativa). Se empleó una velocidad promedio de 0.08 m/s y una amplitud de 2 mm. Las cargas aplicadas fueron de 11.76N (Po = 1.74 GPa) y de 7.84 N (Po = 1.52 GPa). Se realizó mi-croscopía óptica para observar las características de las zonas de desgaste y sus posibles causas de formación. Se obtuvo gráfi camente la variación del coefi ciente de fricción con el número de ciclos. Estos datos se emplearon para determinar con mayor precisión el momento donde se presentaron las primeras señales del des-gaste, adicionalmente se realizaron análisis por Difracción de rayos X (EDS), así como Microscopía Electrónica de Barrido (MEB) y microdureza, que reforzaron las observaciones previas. Fue posible conocer la duración de los recubrimientos y las cusas de su variación. El incremento en la carga de trabajo fue un factor impor-tante en la variación de la vida al desgaste. Sin embargo, es imporimpor-tante considerar otros factores tales como la rugosidad y el espesor de los recubrimientos.
Reference Substrate material Coating Operating conditions Applications Results
Polkar et al., 2006 Austenitic steel TiCN
Temperature: 500 °C Load: 15 N Linear speed: 0.04 m/s Tribometer: pin on disc
Cutt ing tools
The rises in temperature increase the friction coeﬃ cient and wear rates
on TiCN coatings.
Löhr et al., 2006 100Cr6 DLC
Slip rolling friction Po= 1.5-2.3 GPa
Dry condition Tribometer: twin disc
Speed: 390 rpm
Ball bearing races or cages
Acoustic Emission provides an easy solution
for monitoring the wear life of DLC coatings.
Okumiya, 1999 100Cr6 TiN, CrAlN, CrN
Normal load: 50 N Speed: 3 m/s Tribometer: two roller
Ball bearings, gear wheels
No positive eﬀ ect of rolling wear was found.
Carvalho et al., 1998 Tool steel TiN
Tribometer: pin on rig tester
Oil lubricated conditions Load: 0.4 – 1.2 KN Speed: 500 rpm, RCF
Cutt ing tools
The fatigue life is at lower stress levels signifi cantly infl uenced by both the pre-treatment and the fi nal surface roughness of
Singer et al., 1991 M2 Tool steel TiN
Sliding contact Reciprocating sliding
machine Speed: 0.1 – 1 m/s
Load: 2 to 10 N
Cutt ing tools, precision bearings
Wear of TiN took place in two stages. First an air formed oxide layer to
TiN was transferred to the ball, then oxide debris
transferred back to the TiN surface.
Table 1. Features of some previous research on hard coatings
The ball and fl at test specimens were cleaned of any re-sidue oxide layer or machining lubricant by washing in ethanol in an ultrasonic bath (Fisherbrand FB 11020). Subsequently, the ball and disc specimens were dried with hot air. The specimens were placed in the clamps of the test machine. Then the test parameters were in-troduced into the computer, such as: load, frequency and number of cycles. Finally the displacement ampli-tude was selected (2 mm). The maximum contact pres-sure was selected in such a way that wear would be produced with a low number of cycles. A Labview pro-gram was developed to set up the parameters of each
test and collect the data generated, which was basically the friction coeﬃ cient versus time. On the screen it is possible to control the test parameters and follow the progression of the friction during every test. The tests performed with a load of 11.76N were run to 72000 cy-cles and tests with a load of 7.84N were run to 108000 cycles.
This was predetermined with several preliminary tests, to see how many cycles were required to cause damage on the surface coatings. All coatings were tes-ted at the same number of cycles. Not established a fa-ilure criterion to mark the end of the wear life of coating. Table 3 shows the operating conditions of the tests con-ducted. Substrate Material Coating Average Hardness HV Average Roughness
Young´s Modulus GPa (for the steel)
Poisson´s ratio (for the steel)
Coating Thickness μm 4320 steel TiN CrN WC/C Without Coating 1962 995 1258 780 0.25 0.31 0.44 0.35 200 0.3 3 2 3 8620 steel TiN CrN WC/C Without Coating 2507 1057 1261 720 0.37 0.21 0.42 0.32 200 0.3 3 2 3 4140 steel TiN CrN WC/C Without Coating 2248 1023 1147 550 0.21 0.23 0.38 0.30 200 0.3 3 2 3
Table 2. Properties of specimens
tested Test atmosphere
pressure GPa Load N
Frequency Hertz Amplitude mm Cycles 4320 steel TiN CrN WC/C No coating
3 of each coating
C and 45% - 50% relative
1.74 and 1.52 11.74 and
7.84 20 2
72000 and 108000 8620 steel TiN CrN WC/C No coating
3 of each coating
C and 45% - 50% relative
1.74 and 1.52 11.74 and
7.84 20 2
72000 and 108000 4140 steel TiN CrN WC/C No coating
3 of each coating
C and 45% - 50% relative
1.74 and 1.52 11.74 and
7.84 20 2
72000 and 108000
The fi gure 2 shows the case of 4320 steel. It can be seen the diﬀ erence in the friction behaviour for the three coatings. For TiN coating, was observed that the fric-tion coeﬃ cient begins to rise from 500 cycles and for CrN was observed that the friction coeﬃ cient is greater with the minor load, and there is a great variation from 5000 cycles. This was probably caused by the removal of the coating. In the case of the WC/C coating, the fric-tion coeﬃ cients obtained were very similar to those re-ported by other works (Joost et al., 2008; Bonny et al., 2008; Colik et al., 2006; Stewart et al., 2002) and by the supplier of the coatings (Balzers), was obtained a fric-tion coeﬃ cient average between 0.13 and 0.15.
In the fi gure 3 appears the friction behaviour of 8620 steel. For the TiN coating an increase in the friction co-eﬃ cient is seen from 2000 cycles; this may be due to shedding of the coating. For CrN, there is a higher fric-tion coeﬃ cient reaching a value of 0.4 from 1800 cycles. In some cases the friction coeﬃ cient value was lower. For WC/C there were lower values in both load cases obtaining values until 0.1. This may be due to the low coeﬃ cient of friction characteristic of WC/C, allowing a longer life. The shedding of this coating was in the form of small particles, which led to increased friction bet-ween the surfaces in contact. According to this, with the load of 11.76N there is a greater contact pressure and the particles are displaced outside the contact zone, re-ducing the coeﬃ cient of friction, this situation was no presented with the lower load (7.84N) in which, the contact pressure is less, some of the particles were tra-pped between the contact surfaces, increasing in some cases the coeﬃ cient.
The tests with 4140 steel (fi gure 4), show for TiN coating a decrease in the friction coeﬃ cient (0.25) from 5000 cycles. Most of the tests carried out with TiN, after 500 cycles, friction did not change much. It was further observed during some tests that the shedding of small particles occurred as a result of the sliding contact, cau-sing an increase in the friction, because they act as abra-sive bodies between the ball and coating (until 1000 cycles). This was confi rmed with the analysis of wear and optical microscopy, shown later, where there are some indentations and scratches. For CrN coating, the coeﬃ cient of friction turned out very similar for both loads, and no indication was seen when the coating could have been detached. Unlike the TiN coating, no characteristic wear patt ern was seen in the specimen. In all cases with CrN coatings, from 10000 cycles, there
were no considerable variations of friction coeﬃ cient. Likewise it is noted that in most cases, the coeﬃ cient of friction is higher, with a load of 7.84N. For the WC/C coating, there was similarity of the coeﬃ cient of fric-tion, ranging between 0.1 and 0.14 and there were no signifi cant changes. It can be inferred that the test was not suﬃ cient to achieve damage in the coating. One of the tests was continued until 200000 cycles, without sig-nifi cant damage in the coating.
Figure 2. Friction behaviour of coatings in the 4320 steel
Figure 3. Friction behaviour of coatings in the 8620 steel
The wear tests produced wear scars on the fl at steel spe-cimens and steel balls. There were measurable grooves on the fl at specimens. The wear depth of each groove was measured using a Mitutoyo Surftest Profi lometer. As the depth varied along the length of the groove a number of depth measurements (transverse to the leng-th of leng-the groove) were taken. The experimental average depth was taken from these measurements. From this information the volume of a ‘perfect groove’ could be calculated (Green et al., 2005). Wear rates were obtai-ned from the scar profi les (some examples of which are shown in fi gure 5), which determined the size of the scar (depth, width and length). For the balls, wear di-mensions were determined from measurements taken with an optical microscope.
The specifi c wear rates in specimens of the diﬀ erent coatings and substrates are shown in fi gure 6. In the case of TiN, the steel that presented greatest wear was 4320 steel with a load of 7.84 N, then the 8620 steel with 7.84 N and after that the 4140 steel for a load of 11.76 N. The smallest wear rate was with 8620 steel (11.76 N). The behaviour of the wear-load relationship for steels 4320 and 8620 was in agreement with expectations, i.e. higher load, greater wear. This also explains why on the load-friction coeﬃ cient relationship, there was greater detachment of the coating, but the coeﬃ cients of fric-tion were lower. For the CrN coating, it was more diﬃ -cult measure the wear volume to determine the wear rates, because the irregular form of the scar, it was used the average of the scars from the roughness profi les (fi -gure 5). The greatest specifi c wear rate happened in the 4140 steel (11.76 N), and the lowest value was presented in the 4320 steel (7.84 N). For the WC/C coating, the wear was greater in the balls than in the coating (fi gures 6 and 7), due in part to the low coeﬃ cient of friction. In general, the wear rates in the specimens were similar in all substrates and types of load. The wear rates of
subs-trates (without coating) displayed in fi gure 6, indicate excessive wear in the substrate and litt le wear in the balls (fi gure 7). The wear rates in balls are presented in
fi gure 7. For the TiN, the greatest value was presented at the ball in contact with the 4320 steel (11.76 N) after this is the case of 8620 steel with a load of 7.84N and then the 4140 steel with a load of 7.84 N. The lowest wear rate was presented in the 4320 steel (7.84 N). For the balls in contact with CrN, the highest wear rate ha-ppened in the ball against the 4140 steel with a load of 7.84 N. In the balls in contact with WC/C, there are sig-nifi cant variations, especially in those with a load of 7.84N and 108000 cycles. This suggests that in this case, the duration time of the test was more signifi cant rather than the applied load. The greatest wear was presented in the ball against 8620 steel (load of 7.84 N). This
re-fl ects the current application of this coating for cutt ing tools. The balls in contact with substrates, as was expec-ted, the greatest ball wear was presented in the balls against the 4320 steel (700Hv), then the 8620 steel (700Hv) and fi nally in the 4140 steel (550Hv). Greater damage occurs with the implementation of higher loads and not with longer tests.
Figure 5. Roughness profiles
Figure 6. Wear rates in specimens
Optical microscope, SEM and EDS
The fi gures 8 and 9 show some images of the wear scars of the coatings and balls respectively. In the case of TiN, it shows that the wear scar has a regular form, which helped to determine the volume of wear; the brighter areas are exposed substrate. The SEM micrographs (fi -gures 10a and 10b) show the wear scars for 8620 steel with a TiN coating and the characteristics of wear wi-thin the scar. Detachment or complete disappearance of the coating can be observed in some areas. This can also be observed in the EDS analysis shown in fi gure 11a. Other work has shown similar results (De Bruyn et al., 1993).
In the CrN coating, it can be seen that clear scars were not formed as with the other coatings, instead iso-lated areas and irregular wear were seen. The dark areas are still coated and the clear areas are where the substrate material has been exposed (fi gure 8b).
To determine that in some areas the coating was re-moved it was necessary to test hardness, such as that shown for the steel 4320 with a load of 11.76N (fi gure 8e), where the wear scar produced by Vickers indenta-tion appears, and whose measurement corresponded to the substrate (700 HV). The SEM micrograph (fi gure 10c and 10d) shows that wear produced was irregularly shaped in the 4320 steel with a coating of CrN. Figures 10e and 11b show a SEM micrograph and EDS graphic respectively, of 4140 steel with CrN coating, in the fi rst, the clear areas represent removed coating (substrate) and the second shows how the content of Chromium has decreased signifi cantly.
In the WC/C coating, the scar was also produced in a regular form, but narrower than that produced with a TiN coating. The duration of the tests was not suﬃ cient to cause considerable damage in the coating, and what is seen in the fi gures are wear scars but never with a completely detached coating. In the case of the substra-te (without any coating), the wear scars produced were well-defi ned geometrically. A brighter area is visible in the image (fi gure 8c), which indicates a surface polis-hing by the contact with the ball and also severe plastic deformation.
For the balls, all images (fi gure 9) show the wear produced by the contact with diﬀ erent coatings in the 4140 steel substrate. In some cases as can be seen, the scars are big, which also can be verifi ed in the wear
ra-tes (fi gure 7). For the TiN coating, in some cases, adhe-sion of coating material on the ball was observed, presumably particles of TiN, however when making EDS (fi gure 11c), evidence was not found to confi rm this. The diameter of scar in most cases was approxima-tely 1.2 mm. In some cases, grooves were found due to contact with the coating, such as 4320 steel (7.84N) and 8620 steel (11.76N). It may be noted in some situations, the wear scar is uniform (circular), but in most of cases they have an elliptical form or are irregular. This is mainly due to the direction of slip and the applied load, but may also be due to factors related to the adhesion of the coating and possible upset in holding the ball.
In the case of balls in contact with the coating of CrN, most have an almost circular scar and wear was more regular in the surface coating and in the ball. This can be seen clearly in the images (fi gure 9) for the 4140 steel, which show the wear scar with well defi ned ed-ges, without cracks. Within the scars, there are some small dark points, which were formed due to contact with third bodies, like wear particles of the same coa-ting or ball material. In general it was found that there was less wear on the balls in contact with CrN, than with TiN.
When in contact with the WC/C coating, the size of wear scar in the balls is much lower when compared with the previous coatings. The diameter of the scar is in the order of 0.6mm, almost half that of the scars wor-ked with TiN and CrN coatings. As mentioned earlier, referring to the coeﬃ cient of friction and wear rates, this is mainly due to the low coeﬃ cient of friction oﬀ e-red by the WC/C. Even for example in the case of 4140 steel, the scar has a irregular form, with spots that are actually deeper scars, that could also have been caused by the original surface defects on the surface of the ball, which can be seen in the same image (fi gure 9). It is worth mentioning that in the case of this coating, the cycles to which the discs were subjected, were not suﬃ -cient to cause damage in the coating completely. See also fi gures 6 and 7 which show the vast diﬀ erence bet-ween the wear in the coating and in the balls.
Figure 8. Optical microscope of 4320 steel: a) TiN, b) CrN, c) WC/C, d) No coating, e) CrN Hardness test
Figure 10. SEM micrographs of wear scar: a) and b) 8620 steel, TiN coating, c) and d) 4320 steel, CrN coating, e) 4140 steel, CrN coating
Figure 11. EDS graphics: a) 8620 steel specimen with a TiN coating, b) 4140 steel specimen with a CrN coating, c) 100Cr6 steel ball, in contact with a 4320 steel specimen with TiN coating
Sliding wear behaviour of TiN, CrN, and WC/C coatings was evaluated in dry conditions, friction coeﬃ cients, wear rates and SEM micrographs were obtained, as well as EDS analysis, to determine whether there was transfe-rred material of the coating to the ball, and to analyze the degree of wear of the coating on the substrate.
In the case of TiN coating, applied to steels AISI 4320, 8620 and 4140, the images in fi gure 8, show a scar characterized by a failure mechanism initiated by abra-sion. The wear in the coating was caused by contact with the ball. TiN particles removed, joined on the ball, which caused further acceleration of wear. In fi gure 8 can be seen that the mechanism of wear was similar in all tested steels. First there was a high detachment of the coating in the form of small particles, which were an important factor to accelerate the gradual wear of the coating. The particles, in direct contact between the sur-faces, caused noise and vibration, creating instability in the system. This may have led to a rise in temperature in the contact area, further weakening the coating. In most cases the tests were run until the total detachment of the coating, and even appear to wear on the substrate (shiny appearance at the scar) occurred.
In the case of the ball, in this type of coating there was not adherence of TiN on the ball, corroborated by EDS analysis. In some cases uniform wear was not ob-served on the ball, forming irregular areas, perhaps due to the presence of abrasive particles that are displaced from the centre toward the sides. This phenomenon was observed mainly in tests with the load of 11.76N.
In the case of the CrN coating, it was diﬃ cult to identify the mechanism of failure. The wear originated does not follow a traditional patt ern as in the case of other coatings. Uniform wear was not seen and it was diﬃ cult to detect visually the release of the coating. Wear particles were observed to a lesser amount than with the TiN coating. Adhesion of CrN was not obser-ved in the ball. The wear in the ball was uniform and larger compared with TiN and WC/C. This coating had bett er wear resistance than TiN. The CrN coating acts as a repellant to the mechanisms of failure of traditional sliding wear, resulting in small areas of wear of the coa-ting that are isolated and irregularly shaped (fi gure 8). Some tests lasted until 150000 cycles without any chan-ges in the surface or size of the areas of wear. Noise and vibration were not apparent. As can be seen in fi gure 6, wear rates on the ball were greater than in the other coatings, reinforcing the idea of the high wear resistan-ce of the CrN. This coating, acted eﬃ ciently in this type of wear, under the specifi c conditions of the tests
con-ducted, showing litt le wear on the surface of the three tested steels. This explains the recent high use of this type of coating on diﬀ erent applications of mechanical parts subject to sliding wear, including cutt ing tools, guides, dies, and so on.
The WC/C coating showed the best performance in this work. The wear rates of this coating and balls were the lowest of the three coatings employed (fi gures 6 and 7). The low coeﬃ cient of friction (0.15 - 0.2. see fi gure 3) is the most important factor that led to low wear rates. The wear scar apparently shows a detachment of the coating (fi gure 8). However, closer examination shows this is polishing on the surface and the coating is actua-lly intact. In the case of the ball in contact with this coa-ting, fi gure 9 shows that traces of wear are smaller than in the case of other coatings. In trials with this coating, particles did not appear that could act as an abrasive in the contact area and that might have accelerated wear. Under the conditions of the experiments signifi cant wear did not occur in tests are left to run for more than 3 hours (200,000 cycles).
In the experiments outlined in this paper studying sliding wear, TiN and CrN showed a bett er performan-ce in comparison with results obtained previously in RCF tests (Vera et al., 2008). These results showed poor resistances to this kind of wear (RCF), and the coatings rapidly detached, particularly the TiN.
There was no signifi cant diﬀ erence among the three substrates. However, one can see that the results of wear rates and scars seen by optical microscopy and SEM, in most cases, the 4320 steel gives slightly bett er wear performance than the other two. According to the chemical composition of the substrates, the major diﬀ e-rence between them is the content of nickel. This gives the properties of high strength, yield strength greater than carbon steels, high temperature resistance and co-rrosion. The 4320 steel has a high percentage of nickel (1.62 - 2%), which reinforces the veracity of the results achieved.
Substrates AISI 4320, 8620 and 4140 used in this stu-dy showed acceptable properties to resist sliding wear and provide an eﬃ cient alternative for implementation under the conditions used in this work.
• There were no signifi cant changes in the coeﬃ cient of friction between the three substrate materials tested. But signifi cant changes among the three coatings used were found, especially with the WC/C coating.
• In some cases, the variation of the friction coeﬃ -cient against the number of cycles indicated the re-moval of the coating, mainly with the CrN coating. • In most cases, there were no signifi cant variations of the coeﬃ cient of friction between the two loads used in this study, especially with the WC/C coating. • The behaviour of specifi c wear rates for TiN
coa-ting was higher in the specimens and lower in the balls. In the case of CrN and WC/C coatings, the opposite happened.
• The WC/C coating, presented the best wear resis-tance by sliding, when it was tested until 200000 cycles, without substantial damage.
• It is feasible to use these substrates subjected to sli-ding wear, provisli-ding another alternative for the selection of materials in the manufacture of mecha-nical elements subjected to this type of wear.
The work described in this paper has been supported by the Tribology Group, of the University of Sheﬃ eld, UK. The authors acknowledge Balzers Group for the deposition of PVD TiN, CrN and WC/C coatings on ste-el substrates.
Arnell R.D. et al. Tribology: Principles and Design Applications, Mac-millan Education LTD, 1991.
BonnyK., De Baets P., Ost W. Infl uence of Secondary Electro-Conduc-tive Phases on the Tribological Response of Zirconia-Based Compo-sites Against WC-Co Cemented Carbide, Nordtrib, Tampere, Finland, 2008.
Bhushan B., Gupta B.K. Handbook of Tribology: Materials, Coatings and Surface Treatments, McGrawGill, 1991.
Carvalho N.J.M., Huis A.J., In’ T Veld J., De Hosson Th. Interfacial Fatigue Stress in PVD TiN Coated Tool Steels Under Rolling Contact Fatigue Conditions. Surf. Coat. Technology, 105:109-116. 1998.
Celik E., Culha O., Uyulgan B. Assessment of Microstructural and Mechanical Properties of HVOF Sprayed WC-based Cermet Coatings for a Roller Cylinder. Surf. Coat. Technology, 200: 4320-4328. 2006.
De Bruyn K., Celis J.F., Roos J.R. Coating Thickness and Surface Roughness of TiN Coated High Speed Steel in Relation to Coating Functionality. Wear, 166:127-129. 1993.
Green D.A., Lewis R., Dwyer-Joyce R.S. The Wear Eﬀ ects and Mechanisms of Soot Contaminated Automotive Lubricants, IMechE, Part J. Journal of Engineering Tribology, 220:159-169. 2005.
Joost R., Pirso J., Viljus M. The Eﬀ ect of Carbon Content on the Mechanical and Tribological Properties of WC-Co Cemented Carbides, Nordtrib, Tampere, Finland, 2008.
Löhr M., Spaltmann D., Binkowski S. In Situ Acoustic Emission for Wear Life Detection of DLC Coatings During Slip-Rolling Friction. Wear, 260:469-478. 2006.
Okumiya M., Griepentrog M. Mechanical Properties and Tribolo-gical Behaviour of TiN-CrAlN and CrN-CrAlN Multilayer Coatings. Surf. Coat. Technology, 112:123-128. 1999.
Polcar T., Novák R., Siroký P. The Tribological Characteristics of TiCN Coating at Elevated Temperatures. Wear, 260:40-49. 2006.
Singer I.L., Fayeulle S., Ehni P.D. Friction and Wear Behaviour of TiN in Air: the Chemistry of Transfer Films and Debris For-mation. Wear, 149:375-394. 1991.
Srikant-Nekkanty M.E.W. Indentation Damage to Boron Carbide-DLC Coatings with Diﬀ erent Compositions. Surf. Coat. Tech-nology, 183:1-9. 2004.
Stewart S., Ahmed R. Rolling Contact Fatigue of Surface Coatings- A Review. Wear, 253: 1132-1144. 2002.
Sue J.A., Troue H.H. Friction and Wear Properties of Titanium Nitride Coating in Sliding Cont.
About the authors
Edgar Ernesto Vera-Cárdenas. He received the B.S. degree in mechanical engineering (ME) from Instituto Tecnologico de Pachuca in 1995. In 2003, he received his master degree in ME from Instituto Tecnologico de Celaya and his PhD degree in ME from Instituto Politecnico Nacional, in 2009. He was a visiting PhD student at University of Sheﬃ eld, UK, in 2008. He has published research papers in diﬀ erent national and international conferences. Currently he is a research professor at the coordina-tion of mechatronics of the Universidad Politecnica de Pachuca.
Manuel Vite-Torres. He received the B.S. degree in physics from the Faculty of Science of the UNAM, in 1979. He received his PhD degree in applied physics at the Facul-ty of Applied Physics and Nuclear Engineering from the Technical UniversiFacul-ty of Prague, Czech Republic. He is member of the National System of Researchers (SNI) level 1 and active evaluator of CONACYT and Chilean System of Science (CONI-CYT). He has directed over 25 undergraduate thesis and 20 postgraduate thesis. Currently he is a research professor at the SEPI-ESIME-IPN developing projects related to tribology.